PRODUCT DATA SHEET
(Previous date 15.09.2014)
Fontefloor EP Primer - Epoxy primer
|DESCRIPTION||A two-component water-borne epoxy primer.|
Used for dust binding and priming of untreated concrete floors.
Seals the concrete surface and confirms adhesion prior to Temafloor coatings and screeds and Fontefloor paints.
Suitable for priming of damp concrete (relative humidity of the concrete over 97%) surfaces prior to Fontefloor EP 100 epoxy paint.Can be used for patching cracks and holes in concrete.
|Recommended uses||Concrete floor.|
|Features||• Good water vapour permeability.
• The M1 classification for low-emitting building materials has been granted by the Finnish Building Information Foundation RTS.
|Building material emission class||M1|
Coverage on concrete floors is on the average:
Priming 5–7 m2/l
Practical coverage depends on the porosity and evenness of the substrate and on the application method.
|Mixing ratio||Base 1.5 parts by volume 008 4570
Hardener 1 part by volume 008 4571
|Pot-life (+23°C)||Approx. 40 min after mixing (50% thinned).|
|Drying time at 23°C and 50% relative air humidity||
Dust dry after 5 hours
Recoatable after 6 hours
Fully cured after 7 days
Drying and recoating times are related to the film thickness, temperature, the relative humidity of the air and ventilation.
|Solids volume||approx. 66%.|
|Density||1.1 kg / l (mixed).|
|Product code||Base 008 4570 and hardener 008 4571|
|Application conditions||The temperature of the ambient air, surface or coating should not fall below +15ºC during application or drying. Relative humidity of air should not exceed 80%.|
Remove laitance by power grinding or hydrochloric acid etching. Choose the method best suited for the premises. After grinding remove dust carefully with a vacuum cleaner. Hydrochloric acid etching is carried out with diluted hydrochloric acid (1 part concentrated hydrochloric acid, 4 parts water). Rinse with plenty of water. Dry the floor.
Remove all grease, oil, chemicals and other impurities by MAALIPESU detergent. Remove old peeling paint layer by grinding. Clean out pot-holes removing all loose friable material. Open cracks with e.g. an abrasive tool. Remove loose material and dust.
|Priming||Prime with 30–50% thinned Fontefloor EP Primer. Always add the water needed to a ready mixture and stir thoroughly. Pour the mixture onto the floor, apply with a rubber trowel or a roller. Prime once or twice depending on the porosity of the concrete.|
|Patching||Fill holes and cracks with a mixture of unthinned Fontefloor EP Primer and dry, clean sand. Mixing ratio e.g. 1 part by volume of Fontefloor EP Primer mixture and 1–2 parts by volume of sand of grain size 0.1–0.6 mm. Sand the patched areas before finishing.
Note! Concrete surface should always be primed before patching.
|Finishing||Finishing should be done not earlier than 6 hours after the priming. If the primed surface is not overcoated within 48 hours, it should be abraded. Pour the mixture onto the floor, apply with a rubber trowel and level with a roller.
Note! Fontefloor EP Primer adheres also to wet concrete. If there is constant moisture rising from the concrete and Fontefloor EP Primer is topcoated with a non-breathing coating or screed, there is a risk of failure between the primer and topcoat.
|Mixing of components||Mix the correct proportions of base and hardener thoroughly (3–5 minutes) by using a low speed industrial hand drill with a paddle. Insufficient mixing or incorrect mixing ratio will result in uneven drying of the surface, weaken the properties of the coating and risk the success of the application. The resulting emulsion can then be thinned with water to desired application viscosity.|
|Cleaning of tools||Water. Equipment should be cleaned immediately after use before the paint has dried.|
|EU VOC 2004/42/EC-limit value||VOC 2004/42/EC (cat A/j) 140 g/l (2010)
Fontefloor EP Primer: max. VOC < 140 g/l
|HEALTH AND SAFETY LABELLING|
according to Regulation (EC) No. 1272/2008
|Containers are provided with safety labels, which should be observed. Further information about hazardous influences and protection are detailed in individual health and safety data sheets. A health and safety data sheet is available on request from Tikkurila Oyj.|
|Safety data sheet||Fontefloor EP Primer|
|Hardener safety data sheet||Fontefloor EP Primer|
|DECLARATION OF PERFORMANCE||Declaration of Performance EN1504-2|
|The European harmonized productstandard EN 1504-2:2004 defines the requirements for surface protection systems for concrete.
This product is tested and CE-labelled in accordance with the tables 1d, and 1f in the